Elastic Instability of a Crystal Growing on a Curved Surface

 Dulcie Reynolds
 5 months ago
 Views:
Transcription
1 Elastic Instability of a Crystal Growing on a Curved Surface The Harvard community has made this article openly available. Please share how this access benefits you. Your story matters. Citation Published Version Accessed Citable Link Terms of Use Meng, Guangnan, Jayson Paulose, David R. Nelson, and Vinothan N. Manoharan Elastic Instability of a Crystal Growing on a Curved Surface. Science 343 (6171): doi: /science doi: /science February 13, :34:04 AM EST This article was downloaded from Harvard University's DASH repository, and is made available under the terms and conditions applicable to Other Posted Material, as set forth at (Article begins on next page)
2 Elastic instability of a crystal growing on a curved surface Guangnan Meng 1, Jayson Paulose 2, David R. Nelson 1,2 and Vinothan N. Manoharan 2,1 1 Department of Physics, Harvard University, Cambridge MA 2 Harvard School of Engineering and Applied Sciences, Harvard University, Cambridge MA USA One sentence summary: A constant background Gaussian curvature alters crystal growth and favors the formation of anisotropic, ribbonlike domains. Although the effects of kinetics on crystal growth are wellunderstood, the role of substrate curvature is not yet established. We study rigid, twodimensional colloidal crystals growing on spherical droplets to understand how the elastic stress induced by Gaussian curvature affects the growth pathway. In contrast to crystals grown on flat surfaces or compliant crystals on droplets, these crystals form branched, ribbonlike domains with large voids and no topological defects. We show that this morphology minimizes the curvatureinduced elastic energy. Our results illustrate the dramatic effects of curvature on the ubiquitous process of crystallization, with practical implications for nanoscale disorderorder transitions on curved manifolds, including the assembly of viral capsids, phase separation on vesicles, and crystallization of tetrahedra in three dimensions. Since Nicolaus Steno s pioneering work on crystal growth in the 17th century (1), it has been established that the shape of a crystal is a vestige of its growth pathway. Near equilibrium, crystals grown from the melt form compact, faceted This is the authors version of the work. It is posted here by permission of the AAAS for personal use, not for redistribution. The definitive version was published in Science volume 343 on February 7, 2014, DOI: /science To whom correspondence should be addressed. 1
3 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) structures that minimize interfacial area and energy (2, 3), while further from equilibrium, kinetic instabilities (4) permit the formation of crystals with much larger interfacial areas, such as dendrites and snowflakes (5). Less wellunderstood is the role of elastic stress, which can arise from the curvature or lack thereof of the space in which the crystal grows. For example, twodimensional (2D) crystals of spheres on a spherical substrate are strained due to the incompatibility of the preferred triangular lattice packing with the Gaussian curvature of the sphere, which bends the lattice lines. Similarly, in Euclidean threedimensional (3D) space, the absence of curvature frustrates the crystallization of tetrahedra (9, 10). Large, compliant crystals can alleviate this curvatureinduced elastic stress by incorporating topological defects such as grain boundary scars (11, 12) or pleats (13) in the ground state. But for rigid crystals on curved manifolds, for which topological defects such as dislocations have large core energies, the increase of elastic stress with crystal size can also affect the growth process, such that the ground states may be inaccessible. The effects of curvature on the growth pathways are potentially important for analogous processes involving the ordering of identical subunits in curved spaces, such as the assembly of viral capsids (14), filament bundle packing (15), selfassembly of molecular monolayers (16), functionalization of nanoparticles (17), and the growth of solid domains on vesicles (18, 19, 20). We use confocal microscopy to examine the structures of rigid, 2D colloidal crystals growing on the inside walls of highly curved spherical water droplets (Fig. 1A). The particles start in the interior of the droplet, but over a short time nearly all of them attach to the droplet surface through a depletion attraction (6). Once at the interface, the particles attract one another through the same interaction. The short range of the attraction creates a wide coexistence region (Fig. S1) between a lowdensity 2D fluid and a rigid, brittle crystal phase that, unlike the 2D crystals made from repulsive particles (11, 12, 13), cannot easily deform to cover the entire droplet. Because the high interfacial tension of the oilwater interface precludes distortion of the enclosing spherical droplets, and the depletion attraction confines particles to the droplet interface, the crystals are forced to adopt the curvature of the droplet as they grow. This constraint has a dramatic effect on the crystal structures observed at long times: whereas 2D crystals grown on flat surfaces are compact, crystals grown on spherical surfaces are composed of slender, singlecrystal segments that wrap around the droplets, as seen in Fig. 1B. In droplets with higher surface coverage, the thin segments, which we call ribbons, join together to form branched patterns with voids and gaps between them. If these crystals were on flat surfaces, the voids could be filled by additional particles. But the parallel transport caused by the Gaussian curvature forces the crystalline directions to be mismatched at the void borders (Fig. 2A), making it 2
4 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) A C Water droplet R Oil 1.0 µm Polystyrene 80 nm poly(nipam) U m ~4k B T U m >10k B T B R > 2 mm 10 µm R=5.5 µm R=7.2 µm R=9.4 µm R=11.8 µm R=17.6 µm Figure 1: (A) Rigid and brittle colloidal crystals form on the interior surfaces of spherical waterinoil droplets encapsulating an aqueous mixture of 1.0 µm polystyrene (PS) spheres and 80 nm poly(nipam) particles (6). The small particles induce depletion attractions (7,8) between the PS spheres with a strength of about 4 k B T, where k B T is the thermal energy. The depletion force also binds the particles to the interface with a strength of about 10 k B T (6). The range of attraction in both cases is about 80 nm, or about 8% of the PS sphere diameter. A surfactant barrier prevents the large spheres from breaching the interface (6). (B) Representative confocal fluorescence micrographs of crystals grown for a few hours on droplets of various curvatures. Radii of curvature R are noted below micrographs; dotted circles show the droplet surfaces, determined by fitting a spherical model to the particle positions. We use a very large droplet (R > 2 mm) to approximate a flat surface. 3
5 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) A 1 Area A Perimeter L 1 5 µm 2 2 B Frequency flat crystals (R > 2 mm) 10 curved crystals (4.1 µm < R < 46.8 µm) Circularity C Figure 2: (A) From the 3D positions of the particles (red dots), we digitally flatten the curved crystals (6), showing that they are single grains with no topological defects. Arrow (1) shows an apparent grain boundary that is actually a row of vacancies, while arrow (2) shows a void that arises because the curvature bends the lattice vectors. (B) Histograms show that the values of the dimensionless circularity C = 4πA/L 2, measured using morphological image operations (6), are in general much lower for crystals grown on curved surfaces (dark blue, 335 domains) than for crystals grown on nearly flat surfaces (light blue, 187 domains). impossible to continue the crystal without introducing topological defects. Such defects are, however, absent in our system, in contrast to curved crystals made from repulsive particles (11, 12, 13). As we show by digitally unwrapping the crystal structures (Fig. 2A), each crystal is a single grain, and the only defects are vacancies. Morphologically, these structures resemble dendritic crystals. We quantify the morphology using two metrics: the circularity, a measure of the perimetertoarea ratio, and the fractal dimension, a measure of anisotropy. Crystals grown on curved surfaces have much lower circularity (Figs. 2B and S2) and fractal dimension (Fig. S3) than the compact crystals formed on flat surfaces. In flat space, crystals with such large interfacial energies can only result from kinetic instabilities. Here, however, such instabilities are unlikely to be the cause of the anisotropy, since we do not observe dendritic crystals forming on flat surfaces under growth conditions that are otherwise identical to the curved ones (Figs. 1B and 2B). Kinetic instabilities occur when the diffusion of particles along the crystalfluid interface is slow compared to the growth rate. This happens when the domain size is comparable to the MullinsSekerka wavelength λ s (21, 22), which is only 4
6 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) weakly affected by curvature (6). We estimate λ s to be at least 100 µm (6), much larger than the typical width (25 µm or less) of our curved crystals. We therefore exclude kinetic instabilities as the cause of the morphology. We can also exclude kinetic effects arising from fluidfluid coexistence, since our system is far from the metastable fluidfluid critical point (6). The remaining possibility is an elastic instability. A continuum model shows that such an instability occurs because the crystal must compress as it grows larger, owing to the Gaussian curvature of the growth surface. Consider forcing a flat, discshaped crystal of diameter a onto a sphere with radius R. For domain sizes comparable to the sphere radius or smaller, the change in circumference or, equivalently, the elastic strain scales as (a/r) 2, so that the net free energy change, including the elastic energy cost, to form a circular solid domain on a curved surface is (6,23) G(a) = γ (πa) f πa2 4 + π Y a6 R 4, (1) where Y is the 2D Young s modulus, γ the line tension and f the chemical potential difference between the coexisting solid and fluid phases. On flat substrates (R ), the elastic energy vanishes, and crystallites larger than a critical nucleus size a c = 2γ/ f can grow isotropically without limit (dashed line in Fig. 3A). But on curved substrates, the elastic energy increases with domain size a, as measured along a geodesic. Isotropic growth becomes unfavorable beyond a critical size a ( f /Y ) 1/4 R (solid line in Fig. 3A). This restriction on isotropic growth is the origin of the elastic instability (24). The predictions of this simple model are consistent with our measurements of the maximum isotropic domain size, which scales linearly with R (Fig. S4A). Although the crystal could grow larger by incorporating topological defects (25, 26), the short range of the attraction in our system makes such defects energetically costly. Geometry dictates that some interparticle distances near a fivefold or sevenfold defect are larger than the interaction range, effectively breaking the corresponding bonds. Incorporating a fivefold defect, for example, breaks five bonds. This explains the observations in Fig. 2: the stiffness of the potential favors tearing rather than stretching to accommodate stress. Thus if the crystal is to continue to grow, it must do so by increasing its perimetertoarea ratio. It must grow anisotropically. More specifically, the crystal should transition from a disk to a ribbon, or multiple ribbons, when its size exceeds a. This behavior arises because the elastic energy of a ribbon scales with the fifth power of the width w but only linearly in the length l (23, 27). The net free energy change of forming a ribbonlike crystalline domain is: G(w,l) γ 2(l + w) f lw Y w5 l R 4. (2) 5
7 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) A G curved surface B G 0 0 ac a* a 0 flat surface 0.5 l/r w/r Figure 3: A continuum model shows that the elastic stress restricts isotropic domain growth to a maximum size a. The crystal can escape this restriction by growing anisotropically. (A) Free energy G(a) for isotropic growth of a circular crystal of size a on a flat surface (gray dashed line) and a surface with Gaussian curvature (blue solid line). (B) Free energy G(w,l) of formation of a ribbonshaped domain with width w and length l. The (overdamped) crystal growth follows the gradient flow (arrows) on the energy landscape. This energy function is shown as a landscape in Fig. 3B. By maintaining a constant width set by the curvature in the later stages of growth, the crystallite can grow to arbitrarily large lengths, limited only by the number of particles and the area available for growth. The anisotropic growth allows the crystal to avoid the size restriction imposed by elastic energy at the modest cost of a larger interfacial energy. To test this model, we measured the dynamics of growth in single domains, as shown in Fig. 4A and Movie S1. We find that a crystal first grows isotropically until it reaches a critical size, then grows anisotropically, increasing its length while maintaining a much smaller but constant width. Examination of the final crystal shapes for several hundred droplets (Fig. 4B and S4B) shows that the length of the domains can grow to several times the droplet radius, while the width is restricted to a fraction of the radius of curvature. The nearconstant value of w/r seen in Fig. 4 qualitatively agrees with our model, which predicts that the elastic stress limits the width to w R, whereas l can increase without penalty. By fitting the model to the observed domain widths, we extract an effective spring constant for the interparticle interaction that is consistent with theoretical and independent experimental estimates (6), again lending support to the model. The observation of the final, branched crystal shapes is also consistent with our physical picture. A domain can extend its length along any of the three crystallographic axes. If it changes its growth axis, it will bend by ±60, and if it grows in two directions at once, a branch forms. All of these growth patterns are roughly equivalent energetically, as long as the width of the growing section remains less than the critical width dictated by elasticity and curvature. Hence we expect to 6
8 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) A Domain Dimension (µm) min 150 min 190 min 240 min Domain length l Domain width w B w/r Time (minute) w=l l/r Figure 4: (A) Measurements of domain length l (black) and width w (gray) as a function of time for a droplet with R = 18 µm (6). Images of domain morphologies at various times are shown at top (see also Movie S1). The transition from isotropic to anisotropic growth occurs at about 100 minutes. (B) Distribution of l and w, both normalized to the radius of curvature R, for curved crystals. The dashed line marks the isotropic regime where w = l. w/r is roughly constant, in agreement with the model. 7
9 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) see, and do see, changes in direction and branches in the domains. The branches can also arise from the merger of crystallites that have nucleated independently. The branched structures resulting from such mergers maintain their curvaturedependent width w in each section (see Movies S2, S3, and S4). The voids in these structures persist because the crystal directions are mismatched in adjacent sections of the crystal. In contrast, crystallites on flat substrates have no width restriction or curvatureinduced mismatch and can therefore easily merge into isotropic shapes. We conclude that anisotropic crystal growth, usually a result of a kinetic instability, can also occur by slow growth under the geometric constraint of Gaussian curvature. Our results illustrate a generic route for the growth of rigid, defectfree structures in curved spaces. This route may be particularly relevant to nanoscale substrates, where the curvature is appreciable on molecular length scales. For example, solid domains consisting of narrow stripes radiating outward from a circular core have been observed in diverse systems, from phases on lipid vesicles (20) to metal coatings on nanoparticles (17). Our analysis suggests that the width of the stripes and the core size should be determined by the interplay between curvature, elasticity and bulk energy. A similar interplay may affect the assembly pathways of viral capsids. Recent in vitro experiments (28) show that capsids can assemble following a twostep mechanism analogous to our crystallization process: the capsid proteins first attach to a substrate (an RNA molecule) and then bind together into an ordered shell. The intermediate states of this process, long a subject of speculation (14), might contain voids that, like those in our curved crystals, help the capsids avoid excess elastic stress (29, 30). Similar rules may govern other crystallization and packing problems where global geometry is incompatible with local lattice packing. For example, crystallization of tetrahedra is frustrated in flat (Euclidean) 3D space (9). However, logs and helices of tetrahedra are prevalent in firstorder phase transitions of tetrahedra from disordered to dense quasicrystalline phases (10). The existence of these structures, which were first described by Bernal (31), may reflect a similar physical principle, in which growth along one dimension allows a crystal to escape the restrictions of geometrical frustration. 8
10 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) References and Notes 1. N. Steno, The prodromus of Nicolaus Steno s dissertation concerning a solid body enclosed by process of nature within a solid; an English version with an introduction and explanatory notes by John Garrett Winter (MacMillan, London, 1916). 2. I. Sunagawa, Crystals: Growth, Morphology, & Perfection (Cambridge University Press, 2005). 3. A. T. Skjeltorp, Visualization and characterization of colloidal growth from ramified to faceted structures, Physical Review Letters 58, 1444 (1987). 4. J. S. Langer, Instabilities and pattern formation in crystal growth, Reviews of Modern Physics 52, 1 (1980). 5. K. G. Libbrecht, The physics of snow crystals, Reports on Progress in Physics 68, 855 (2005). 6. Materials and methods are available as supporting material on Science Online. 7. S. Asakura, F. Oosawa, On interaction between two bodies immersed in a solution of macromolecules, The Journal of Chemical Physics 22, 1255 (1954). 8. R. Roth, B. Götzelmann, S. Dietrich, Depletion forces near curved surfaces, Physical Review Letters 83, 448 (1999). 9. D. Nelson, F. Spaepen, Polytetrahedral order in condensed matter, Solid State Physics  Advances in Research and Applications 42, 1 (1989). 10. A. HajiAkbari, M. Engel, A. S. Keys, X. Zheng, R. G. Petschek, P. Palffy Muhoray, S. C. Glotzer, Disordered, quasicrystalline and crystalline phases of densely packed tetrahedra, Nature 462, 773 (2009). 11. A. R. Bausch, M. J. Bowick, A. Cacciuto, A. D. Dinsmore, M. F. Hsu, D. R. Nelson, M. G. Nikolaides, A. Travesset, D. A. Weitz, Grain boundary scars and spherical crystallography, Science 299, 1716 (2003). 12. P. Lipowsky, M. J. Bowick, J. H. Meinke, D. R. Nelson, A. R. Bausch, Direct visualization of dislocation dynamics in grainboundary scars, Nature Materials 4, 407 (2005). 13. W. T. M. Irvine, V. Vitelli, P. M. Chaikin, Pleats in crystals on curved surfaces, Nature 468, 947 (2010). 9
11 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) 14. W. H. Roos, R. Bruinsma, G. J. L. Wuite, Physical virology, Nature Physics 6, 733 (2010). 15. I. R. Bruss, G. M. Grason, Noneuclidean geometry of twisted filament bundle packing, Proceedings of the National Academy of Sciences 109, (2012). 16. G. A. DeVries, M. Brunnbauer, Y. Hu, A. M. Jackson, B. Long, B. T. Neltner, O. Uzun, B. H. Wunsch, F. Stellacci, Divalent metal nanoparticles, Science 315, 358 (2007). 17. H. Bao, W. Peukert, R. K. Taylor, Onepot colloidal synthesis of plasmonic patchy particles, Advanced Materials 23, 2644 (2011). 18. R. Lipowsky, The conformation of membranes, Nature 349, 475 (1991). 19. J. Korlach, P. Schwille, W. W. Webb, G. W. Feigenson, Characterization of lipid bilayer phases by confocal microscopy and fluorescence correlation spectroscopy, Proceedings of the National Academy of Sciences 96, 8461 (1999). 20. A. Bandekar, S. Sofou, Floretshaped solid domains on giant fluid lipid vesicles induced by ph, Langmuir 28, 4113 (2012). 21. W. W. Mullins, R. F. Sekerka, Morphological stability of a particle growing by diffusion or heat flow, Journal of Applied Physics 34, 323 (1963). 22. W. W. Mullins, R. F. Sekerka, Stability of a planar interface during solidification of a dilute binary alloy, Journal of Applied Physics 35, 444 (1964). 23. S. Schneider, G. Gompper, Shapes of crystalline domains on spherical fluid vesicles, Europhysics Letters 70, 136 (2005). 24. A. Y. Morozov, R. F. Bruinsma, Assembly of viral capsids, buckling, and the AsaroGrinfeldTiller instability, Physical Review E 81, (2010). 25. Y. Chushak, A. Travesset, Solid domains in lipid vesicles and scars, Europhysics Letters 72, 767 (2005). 26. D. R. Nelson, Defects and Geometry in Condensed Matter Physics (Cambridge University Press, 2002). 27. C. Majidi, R. S. Fearing, Adhesion of an elastic plate to a sphere, Proceedings of the Royal Society A: Mathematical, Physical and Engineering Science 464, 1309 (2008). 10
12 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) 28. R. F. Garmann, M. ComasGarcia, A. Gopal, C. M. Knobler, W. M. Gelbart, The assembly pathway of an icosahedral singlestranded RNA virus depends on the strength of intersubunit attractions, Journal of Molecular Biology advance online publication (2013). 29. W. Klug, W. Roos, G. Wuite, Unlocking internal prestress from protein nanoshells, Physical Review Letters 109, (2012). 30. A. Luque, D. Reguera, A. Morozov, J. Rudnick, R. Bruinsma, Physics of shell assembly: Line tension, hole implosion, and closure catastrophe, The Journal of Chemical Physics 136, (2012). 31. J. D. Bernal, The Bakerian lecture, The structure of liquids, Proceedings of the Royal Society of London. Series A. Mathematical and Physical Sciences 280, 299 (1964). 32. P. Robert, Temperaturesensitive aqueous microgels, Advances in Colloid and Interface Science 85, 1 (2000). 33. J. W. Goodwin, J. Hearn, C. C. Ho, R. H. Ottewill, Studies on the preparation and characterisation of monodisperse polystyrene laticee, Colloid & Polymer Science 252, 464 (1974). 34. J. C. Crocker, D. G. Grier, Methods of digital video microscopy for colloidal studies, Journal of Colloid and Interface Science 179, 298 (1996). 35. G. Meng, N. Arkus, M. P. Brenner, V. N. Manoharan, The FreeEnergy landscape of clusters of attractive hard spheres, Science 327, 560 (2010). 36. A. D. Dinsmore, E. R. Weeks, V. Prasad, A. C. Levitt, D. A. Weitz, Three Dimensional confocal microscopy of colloids, Applied Optics 40, 4152 (2001). 37. E. Jones, T. Oliphant, P. Peterson, et al., SciPy: Open source scientific tools for Python, (2001 ). 38. E. R. Dougherty, R. A. Lotufo, Handson morphological image processing (Spie Press, 2003). 39. H. Xia, P. G. Tucker, Proceedings of the 18th International Meshing Roundtable (SpringerVerlag, 2009), pp A. Vrij, Polymers at interfaces and the interactions in colloidal dispersions, Pure and Applied Chemistry 48, 471 (1976). 41. W. B. Russel, D. A. Saville, W. R. Schowalter, Colloidal Dispersions (Cambridge University Press, 1992). 11
13 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) 42. M. Dijkstra, Phase behavior of hard spheres with a shortrange yukawa attraction, Physical Review E 66, (2002). 43. P. Bolhuis, M. Hagen, D. Frenkel, Isostructural solidsolid transition in crystalline systems with shortranged interaction, Physical Review E 50, 4880 (1994). 44. J. SerranoIllán, G. Navascués, E. Velasco, L. Mederos, Selfconsistent nonperturbative theory: Treatment of colloidaltype interactions, The Journal of Chemical Physics 119, 1510 (2003). 45. T. Chou, D. R. Nelson, Dislocationmediated melting near isostructural critical points, Physical Review E 53, 2560 (1996). 46. A. Santos, M. López de Haro, S. Bravo Yuste, An accurate and simple equation of state for hard disks, The Journal of Chemical Physics 103, 4622 (1995). 47. H. Reiss, H. L. Frisch, J. L. Lebowitz, Statistical mechanics of rigid spheres, The Journal of Chemical Physics 31, 369 (1959). 48. E. Helfand, H. L. Frisch, J. L. Lebowitz, Theory of the two and onedimensional rigid sphere fluids, The Journal of Chemical Physics 34, 1037 (1961). 49. J. A. Zollweg, G. V. Chester, P. W. Leung, Sizedependent properties of twodimensional solids, Physical Review B 39, 9518 (1989). 50. M. Engel, J. A. Anderson, S. C. Glotzer, M. Isobe, E. P. Bernard, W. Krauth, Harddisk equation of state: Firstorder liquidhexatic transition in two dimensions with three simulation methods, Physical Review E 87, (2013). 51. H. S. Seung, D. R. Nelson, Defects in flexible membranes with crystalline order, Physical Review A 38, 1005 (1988). 52. P. R. t. Wolde, D. Frenkel, Enhancement of Protein Crystal Nucleation by Critical Density Fluctuations, Science 277, 1975 (1997). 53. J. Lutsko, G. Nicolis, Theoretical Evidence for a Dense Fluid Precursor to Crystallization, Physical Review Letters 96, (2006). 54. J.P. Hansen, I. R. McDonald, Theory of simple liquids (Access Online via Elsevier, 1990). 55. D. G. Chae, F. H. Ree, T. Ree, Radial Distribution Functions and Equation of State of the HardDisk Fluid, The Journal of Chemical Physics 50, 1581 (1969). 12
14 G. Meng, J. Paulose, D. R. Nelson, V. N. Manoharan, Science 343: 634 (2014) 56. G. Tarjus, F. Sausset, P. Viot, Statistical mechanics of liquids and fluids in curved space, arxiv preprint arxiv: (2010). 57. S. Lishchuk, Equation of state of the harddisk fluid on a sphere from Percus Yevick equation, Physica A: Statistical Mechanics and its Applications 369, 266 (2006). 58. L. D. Landau, L. P. Pitaevskii, E. Lifshitz, A. M. Kosevich, Theory of Elasticity, Third Edition: Volume 7 (ButterworthHeinemann, 1986). 59. We thank Frans Spaepen for helpful discussions. We acknowledge support from the Harvard MRSEC, supported by the National Science Foundation under grant number DMR See Supplementary Materials for additional data. Supporting Online Material Materials and Methods Figs. S1 to S4 References (3258) Movies S1 to S4 13
15 Supplementary Materials for Elastic instability of a crystal growing on a curved surface Guangnan Meng, 1 Jayson Paulose, 2 David R. Nelson, 1,2 Vinothan N. Manoharan 1,2 1 Department of Physics, Harvard University, Cambridge MA USA 2 Harvard School of Engineering and Applied Sciences, Harvard University, Cambridge MA USA To whom correspondence should be addressed; This PDF file includes: Materials and Methods Supplementary Text Figs. S1 to S4 Captions for Movies S1 to S4 Full reference list Other Supplementary Materials for this manuscript includes the following: Movies S1 to S4 1
16 Materials and Methods 1 Preparation of colloidal particles The aqueous colloidal suspension consists of two types of particles, large polystyrene (PS) spheres and small poly(n Isopropylacrylamide) (poly(nipam)) spheres. The poly(nipam) spheres induce a depletion force between the larger spheres, causing them to attract one another and stay near the wateroil interface. We used precipitation polymerization (32) to synthesize the poly(nipam) hydrogel particles. 2.0 g of N Isopropylacrylamide (NIPAM, monomer, 99%, Acros Organics), 0.1 g N,N Methylenebisacrylamide (crosslinker, 99%, Promega), and 0.19 g ( 6.6 mm) sodium dodecyl sulfate (SDS, 99%, EMD Chemicals) were dissolved in 94 ml deionized (DI) water (MilliQ synthesis grade, Millipore). The solution was stirred and heated to 70 C under nitrogen for 30 minutes to remove extra oxygen in the solution. 60 mg of potassium persulfate (KPS, initiator, 99%, Acros) were dissolved in 4 ml DI water and loaded into the reactor to start the polymerization reaction. The reaction ran for 4 hours. Afterward, the poly(nipam) hydrogel particles were cleaned by dialysis against DI water for seven days, with water changes every 24 hours. The hydrodynamic diameter of our particles, as measured by a Zetasizer Nano ZS (Malvern Instruments), was 80 nm at 20 C and 40 nm at 40 C in DI water. Samples observed with confocal fluorescence microscopy were prepared using 1.0 µm fluorescent sulfate latex PS particles (FluoSpheres sulfate microspheres, 1.0 µm, red fluorescent (580/605), Molecular Probes, Cat. No. F8851, polydispersity (standard deviation in particle diameter)=3%). Before using, we cleaned the particles in DI water by repeated centrifugation and redispersion. Samples observed using confocal reflection microscopy were prepared using 0.6 µm nonfluorescent sulfate PS particles, synthesized by surfactantfree emulsion polymerization (33). 15 ml of styrene (monomer, 99%, SigmaAldrich) and 146 ml DI water were mixed and gently stirred by a magnetic stir bar at 200 rpm, then heated to 70 C under nitrogen for 30 minutes g of KPS were dissolved in 4 ml DI water and loaded into the reactor to start the polymerization reaction. The reaction ran for 20 hours. Afterward, the PS particles were cleaned by filtration and repeated centrifugation (3,000g for 1 hour) and redispersion in DI water. The diameter of our particles, as measured through optical microscopy (Eclipse TE2000, Nikon Corp.), was 0.6 µm. In brief, a drop (about 10 µl) of colloidal suspension was dried on a glass coverslip so that the particles formed a singlecrystalline monolayer. We then used image analysis (34) to locate the centers of individual particles in a focused optical micrograph. The particle size was determined by the first peak of the pair distance distribution, calculated from a few thousand particles within the singlecrystalline monolayer. 2 Emulsion preparation The aqueous (internal) phase of the emulsions contained a mixture of PS particles (either 1.0 µm fluorescent PS or 0.6 µm plain PS) and 80 nm poly(nipam) hydrogel particles in water. The concentration of PS varied; the concentration of poly(nipam) was 1.0% w/w, with an estimated volume fraction of φ s 25% at 20 C). 15 mm NaCl were added to screen the electrostatic repulsion between the PS particles, and 0.1% w/w Pluronic P123 (BASF) and 0.25% w/w Pluronic F108 (BASF) surfactant were added to stabilize the PS particles in the solution (35). The surfactants also prevented the PS particles from penetrating the wateroil interface, thus ensuring that the interaction 2
17 between the particles was mediated entirely by the solution conditions inside the droplet, and not by interfacial effects such as capillary forces. To prepare the emulsion, we added 100 µl of aqueous solution to 2 ml silicone oil (Alfa Aesar, Cat. No. A12728) in a glass vial and emulsified using a vortex mixer (VWR). The average size of the emulsified droplets was roughly controlled by the vortexing speed and time, and was between 20 and 50 µm after vortexing at 1,500 rpm for 30 seconds. 3 Sample cell preparation and loading Sample cells were prepared from siliconetreated cover slips. The silicone prevented the droplets from wetting and spreading on the cover glass. The cover slips (22 22 mm, No.1, VWR) were spincoated at 4,000 rpm for 30 seconds with a 10% w/w solution of silicone (10:1 mixture of base and curing agent of SYLGARD 184, Dow Corning Corporation) in cyclohexane. The coated cover slips were left in covered petri dishes at room temperature (22 C) for 24 hours, during which time the silicone coating cured to form transparent, hydrophobic films a few micrometers thick. The emulsion was then loaded between two treated cover slips. The inner edges of the glass cell were sealed with high vacuum grease (Dow Corning) of about 300 µm thickness, and the outer edges were sealed by epoxy (5 Minute Epoxy, Devcon) to prevent solvent evaporation. We waited at least 15 minutes for the glue to be fully cured before observing the samples. For measurements of the crystal structures at long times, we equilibrated the samples at room temperature (22 C) for at least 24 hours before observations. 4 Confocal microscopy observation We used a laser scanning confocal microscope (Leica TCS SP5 II, Leica Microsystems) equipped with an oil immersion objective (100X, N.A.=1.4 or 63X, N.A.=1.4) to observe the three dimensional (3D) structures of the crystals (36). We did not need to indexmatch the particles to the medium, since there was only a monolayer of colloidal particles at the interface. We used different observation modes depending on which PS particles were used to prepare the sample. a. Confocal fluorescence microscopy for 1.0 µm fluorescent PS particles. Laser light with a wavelength of 543 nm was used to excite the fluorophores in the PS particles, and emitted light was collected at 605 nm. The figures of the main text show confocal fluorescent microscopy images. b. Confocal reflection microscopy for nonfluorescent 0.6 µm PS particles. We illuminated the sample with a 543nm laser and collected backscattered light at the same wavelength. Fig. SM1 shows an example of a curved crystal structure formed by 0.6 µm plain PS particles, as imaged using confocal reflection microscopy. To verify that the crystallization of the polystyrene spheres was driven by the weak depletion interaction induced by poly(nipam) particles, we used a microscope objective heater (MTCHLS 025, Bioscience Tools) to heat the immersion microscope objective and control the sample temperature from ambient room temperature up to 35 C with ±0.1 C resolution. Since poly(nipam) depletants change size with temperature, the depletion attraction between PS particles is temperature sensitive: the range and strength decreases as the temperature increases. The sublimation of 3
18 5.0 µm Fig. SM1. Confocal reflection microscopy of curved crystals of 0.6 µm plain PS particles. The image shows the projected view of the 3D dataset along the optical axis. Scale bar, 5.0 µm. the crystals at higher temperature showed that the dominant interaction between the spheres was the depletion interaction caused by the poly(nipam). To show that the particles were bound to the interface by the depletion force, and not by a capillary interaction, we tracked particles in the melting experiments, and found that the PS spheres began to desorb from the interface when the sample was heated (Fig. SM2). When the sample was cooled, the particles readsorbed and crystallized again. Furthermore, in the absence of the poly(nipam) particles, we did not observe the PS particles to stick to the interface. 5 Image processing and analysis methods The experimental data from the confocal microscope is structured as a 3D intensity stack, I(x, y, z), stored as a 3D array of floatingpoint numbers. To extract information about the crystal domains, we used particle finding methods and morphology operations. This analysis was performed on Intelbased desktop computers or Linux clusters (Intel Xeon 64bit, 2670 MHz, 132 GB of RAM; or AMD Opteron 64bit, 2200 MHz, 198 GB of RAM), using the Python language (http://www. python.org) with the SciPy extensions (http://www.scipy.org/) (37 ). 5.1 Particle finding and domain flattening From the confocal stacks I(x, y, z), we used a particle finding algorithm (34 ) to locate the centers of particles in 3D space, as shown in Fig. 2A in the main text, with a precision better than 100 nm. Because the large majority of particles in the solid phase have six neighbors, it is possible to isolate domains of crystalline order on the sphere and flatten them onto an idealized hexagonal lattice while preserving the topology of the network of interparticle bonds. The flattened image is shown in the second panel of Fig. 2A in the main text. To flatten the domains, we first identified nearestneighbor pairs of particles by an adjacency criterion: two spheres were counted as neighbors if their gap distance was within the 100 nm depletion 4
19 # of Particles Inside Droplet Time (s) Fig. SM2. Particle dynamics during a melting experiment. From the confocal microscope stacks comprising each individual frame, we located the centers of several hundred 1.0µm PS particles in 3D. Then we found the center (O) and radius of the droplet (R) at each frame by least squares fitting to the distance between these particles and the droplet surface. During the melting experiment, the number of particles that were 1.0 µm away or more from the droplet surface increased with time, providing evidence that the particles were bound by depletion interactions and not capillary forces. interaction range. We then used the resulting adjacency matrix to build a graph of nearestneighbor relationships. The graph was traversed using a depthfirst search. The first pair of particles were assigned to the (0, 0) and (1, 0) lattice positions of the 2D flattened lattice. Subsequent particles were added to the lattice as follows: for every ith particle visited in the traversal, the angle made by the positions of particles i, i 1, i 2 at i 1 determined the lattice position of the ith point relative to the i 1th particle. For example, if the link between the third and second point of the traversal made approximately a 180 angle with the link between the second and first point, the third point was placed at position (2, 0) on the 2D lattice. In this manner, the flattened version of the domain was constructed particlebyparticle, preserving the local relationships between particles. The algorithm misplaces a few ( 10) particles, especially near the outer edges and gaps in the domain. We corrected these errors by hand. The flattening process was done only to illustrate the crystalline order in Fig. 2 and was not used for any quantitative analysis. 5.2 Morphological operations To extract information about the shapes of the crystalline domains we performed a series of morphological operations (38) on the confocal microscopy image data. We first interpolated the raw data to a resolution of µm per voxel along each direction using a cubic spline. Then, to find solid regions and prepare the data for further analysis, we performed the following operations (see Fig. SM3 for results of each step on the data from a representative experiment): 1. Filtering: to eliminate longwavelength modulation of the brightness due to contrast gradients from the raw confocal stack (Fig. SM3A), we subtract a boxcar average over a volume of extent 2w + 1 in each dimension, where w is the particle radius in pixels (34). We also removed highfrequency noise from the camera and frame grabber by convolving the stack with a Gaussian kernel of width 1 voxel (34). Fig. SM3B shows the filtered stack after these two operations. 5
20 A B C 10 µm D E F Fig. SM3. Morphological operations before further analysis (images show zaxis projections of 3D arrays). (A) Original confocal stack; (B) Contrast gradients and highfrequency noise removed; (C) Thresholding applied to convert stack to binary array; (D) Closing operation to fill in voids; (E) Points within 0.3 µm of the droplet surface isolated; (F) Euclidean distance transform applied. Scale bar, 10 µm. 2. Thresholding: We then binary thresholded the filtered stack, setting all voxels above a threshold intensity to 1 and setting all other voxels to 0. The threshold was chosen to preserve particles but eliminate lowintensity, unwanted features, such as light scattered from the droplet interface. This process results in a binary array where 1 corresponds to a region in space occupied by part of a PS particle, and 0 corresponds to empty space. Fig. SM3C shows the binary thresholded stack. 3. Morphological closing: We performed a morphological closing operation (38) on the thresholded, binary array. This fills in all voids smaller than a single particle, and in particular fills in the regions between closelypacked particles, converting regions of crystallized particles into nearly featureless, continuous solid domains. Fig. SM3D shows the coarsegrained stack. 4. Paring: We pared down the continuous solid domains to a uniform thickness to completely eliminate singleparticle features and enable estimation of domain lengths and widths from voxel counts at later stages. First we found the center and radius of the sphere that minimizes the mean squared distance of the 1 voxels from its surface. The resulting sphere provided the best estimate of the oilwater interface, which is not directly imaged. We isolated all voxels within a finite width of 0.6 µm of the droplet surface and discarded the rest. In this way, all domains had the same thickness perpendicular to the droplet surface. Fig. SM3E shows the pared stack. 6
21 By counting the number of voxels in each pared domain, we could estimate the size of the domain. We restricted our shape analysis to domains that covered an area corresponding to ten or more particles. 5. Euclidean distance transform (EDT): The EDT replaces each 1 voxel with the Euclidean (real space) distance from that voxel to the closest 0 voxel that lies on the droplet surface. Knowing the radius of the spherical droplet allows us to convert this Euclidean distance to a geodesic distance from each point to its closest boundary along the surface of the sphere. Fig. SM3F shows the EDT transformed stack. 5.3 Domain shape analysis We characterized the shapes of the largest crystalline domain from each droplet using several different metrics, as described below, starting from various stages of our image analysis procedure Circularity The circularity C = 4πA/L 2 measures the perimetertoarea ratio a solid domain, where A is the domain area and L is the perimeter length. C measures the compactness of a solid domain relative to a disc on a planar surface (for which C = 1). The smaller C, the more anisotropic the domain. Both area and perimeter were measured from filtered coarsegrained stacks such as the one shown in Fig. SM3E. The domain area A was measured by counting the number of voxels within the domain: A # of voxels in domain Volume per voxel Transverse thickness of domain, (3) where the volume per voxel is (1.25 µm) 3 (see Section 5.2). The domain perimeter L was measured by counting the number of voxels within a distance t of the boundary. To smooth out features on the perimeter smaller than the scale of the particles, we chose t to be the particle diameter. The number of voxels within one particle diameter of the boundary was obtained from the EDT: L Number of voxels with (EDT < particle diameter) Volume per voxel Transverse thickness of domain Particle diameter. (4) These estimates of the area and perimeter for individual domains were used to calculate the circularity of crystal domains reported in Fig. 2C of the main text and Fig. S Mass dimension Another measure of the domain anisotropy is the mass dimension of the domains. The mass function m(r) of a domain is the amount of material within a geodesic distance r of a central point. The mass dimension β is the exponent that describes the scaling of m(r) with r: m(r) r β. It reflects the degree of compactness of a shape: a disc has mass dimension β = 2, while an extended object such as a long, narrow rectangle, or a starfish with long arms of nearly constant width, has mass dimension β = 1. On a sphere, the mass dimension is close to 2 for discshaped domains as long as their size is small compared to the sphere radius; it is 1 for long ribbons with width smaller than the sphere radius. 7
22 10 5 m~r 0.82 m(r) (a.u.) 10 4 m~r 2.02 r 10 3 m(r) 1 10 r (µm) Fig. SM4. Example of a mass dimension measurement for a single domain. The mass m(r) is estimated as the number of voxels within a geodesic distance r of the largest inscribed disc center (white dot), with r incremented by 1.0 µm between data points (concentric circles in schematic). Fitting a contiguous pair of line segments to the plot gives r I = 5.7 µm for the radius separating the inner and outer regions (see text), and the mass dimension estimates of 2.02 (red line) and 0.82 (blue line) for the inner and outer regions respectively. We first determined m(r). For each experimental domain we chose the center of the largest inscribed disc (see section 5.3.3) as the origin. The mass was estimated as the number of voxels in the solid region within a geodesic distance r of the origin. To find the mass dimension, we fit the logm(r) versus logr data to two contiguous line segments with independent slopes (Fig. SM4 solid lines). This model is based on the expected behavior of the mass dimension β for an anisotropic or branched domain (inset of Fig. SM4): at small r, m(r) should grow as r 2 until r becomes comparable to the radius of the largest inscribed disc. At that point m(r) must grow with a different exponent. We used a model with four free parameters to fit the data: the intercept, the two slopes, and the distance r I that separates the inner and outer regions. To ensure that we identify a distinct outer region, we require that r I < r max /2, where r max is the largest value of r within the domain. Domains that fail these test are likely to be compact, with some small regions at the boundaries skewing the value of the outer mass dimension. For such domains, the outer mass dimension estimate is not reliable, and we assigned the inner mass dimension to the outer region as well. We show m(r) and a histogram of the mass dimension for several hundred domains in Fig. S Inscribed disc diameter, domain length, and domain width We measured the inscribed disc diameter a of curved crystal solid domains from the EDT stack, such the one shown in Fig. SM3F. For a given domain, a is the diameter of the largest possible disc that fits completely within the solid domain. It is simply twice the largest value of the EDT. The center of the largest inscribed disc is the point in the domain with this value. Fig. SM5A shows the center and edge of the inscribed disc for the largest domain from Fig. SM3F. To characterize the length and width of the noncompact and often branched or zigzag shapes of the equilibrated crystallites, we used the morphological skeleton, the set of all points in the domain 8
23 A B Fig. SM5. Morphological measurement of a solid domain. (A) Closeup of the largest domain from the droplet shown in Fig. SM3F. The intensity corresponds to the Euclidean distance transform (EDT). The red dot is the point in the domain with the largest value of the EDT, which corresponds to the center of the largest inscribed disc. The blue circle shows the edge of the largest inscribed disc; the diameter of this circle (twice the largest value of the EDT) was used to estimate a for the domain. (B) Morphological skeleton overlayed on the EDT. The blue and orange points follow ridges in the EDT, approximating the morphological skeleton. The orange points follow the longest contiguous branch, or backbone. with more than one closest point on the boundary. The morphological skeleton is equivalently the set of centers of all circles that are tangent to the domain boundary at two or more points. The skeleton follows points where the Euclidean distance transform (EDT) changes sharply. It corresponds to regions where the Laplacian of the EDT takes on large negative values (39). To estimate the morphological skeleton from the EDT of a domain, we calculated the numerical Laplacian of the EDT at each 1 voxel. We isolated voxels with Laplacian lower than a threshold of 6.4/ µm, corresponding to a change in the EDT by one voxel over a distance of about 1.2 voxels. We then picked a sparse subset of these points, chosen randomly with the restriction that no two points are closer than half a particle diameter, to represent the morphological skeleton (Fig. SM5 B). The value of the EDT at each skeletal point corresponds to the radius of the disc centered at that point that is tangential to two or more points on the boundary of the domain. Thus it is half the local width of the domain at that point. A typical skeleton contains many branches, some minor branches that connect the main central branch of the skeleton to features along the boundary, and others major branches following the branched shape of the domain itself (Fig. SM5B). To measure the length of a domain, we isolated the longest continuous branch of the skeleton by successively removing the shortest surviving branch until only two endpoints remained in the skeleton. This branch, called the backbone, is highlighted in Fig. SM5B. For a domain that is highly convoluted but does not have any branches, the length of the backbone is a good measure of the extent of anisotropic domain growth. For a domain with multiple major branches, the length of the backbone quantifies the length of the longest section of the domain. The length of the backbone is reported as the domain length l in Fig. 4 of the main text. The average diameter of the central discs along the backbone, weighted by the area of each disc to 9
24 minimize the effects of the tapered regions at the ends of domains, is reported as the domain width w in Fig. 4 of the main text. The inscribed disc diameter a and the domain width w for several hundred domains are shown in Fig. S4. 6 Theoretical methods 6.1 Pair potential Our calculations of the phase behavior and elastic energy rely on a model for the pair potential. This model has two components: a depletion attraction and an electrostatic repulsion. The driving force for the crystallization is the depletion attraction between PS particles and between the particles and the wateroil interface. We modeled the depletion interaction between two PS particles with the AsakuraOosawa depletion theory for a binary spherical mixture (7, 40): U AO (r) = k B T φ s (2a s ) 3 (2a s + 2a l r) 2 (2a s + 2a l + r 2 ) (5) where r is the centertocenter distance between two PS particles, φ s the volume fraction of poly (NIPAM) depletants ( 25%), a l the radius of the large PS particles (a l = 500 nm or 300 nm) and a s the radius of the small poly(nipam) (a s = 40 nm) depletants. The range of the interaction is the diameter of the poly(nipam) depletant 2a s = 80 nm. The strength of the depletion attraction can be calculated when two PS particles are touching r = 2a L : U AO (2a L ) = k B T φ s (1 + 3a l 2a s ) (6) The surfaces of the PS particles have negativelycharged sulfate groups. When two PS particles are close to one other (r 2a l ), there is a screened Coulomb repulsion between them, which modifies the shape of the depletion well at small separation: ( e U DLVO (r) = k B T Z 2 κa l ) 2 e κr λ B (7) 1 + κa l r where Z is the surface charge valence per PS particle, λ B the Bjerrum length, and κ 1 the Debye screening length (41). For our experimental conditions, λ B = 0.7nm, and κ 1 = 2nm. We do not know the surface charge for the 0.6µm plain PS particles, which were synthesized in our lab. For the fluorescent particles, we used samples from several different batches that had different surface charges as reported by the manufacturer. We therefore estimated Z = for the surface charge for these beads, following our previous calculations (35, Supplementary Materials) from similarlysized particles from the same manufacturer. This surface charge is of the same order of magnitude (10 5 ) as the various surface charges reported by the manufacturer for the fluorescent beads. The pair potential between PS particles is the summation of the depletion attraction and Coulomb repulsion: U(r) = U AO (r) +U DLVO (r) = k B T φ ( s (2a s ) 3 (2a s + 2a l r) 2 2a s + 2a l + r ) ( e + k B T Z 2 κa l λ B κa l ) 2 e κr. r The potential is shown in Fig. SM6. We estimate that for our experimental conditions, the strength of the depletion attraction between PS particles, taking into account the electrostatic repulsion, is U m 4k B T. 10 (8)
25 Attractive v(r)/k B T 4 Repulsive 2 Total r/µm Fig. SM6. Pair potential between colloidal spheres with diameter d = 2a L = 1.0 µm. The attractive (AsakuraOosawa) and repulsive (screened Coulomb) components and their superposition are shown. The diameter of the poly(nipam) depletant particles is 80 nm, which sets the interaction range. The depletion attraction between the PS particles and the curved wateroil interface can be estimated in a similar manner (8). The range of the attraction is the same as between the particles, but the strength at contact is twice as large or more: ( U AO(2a L ) = k B T φ s 1 + 3a ) l R 2U AO (2a L ) (9) a s R a l where R is the radius of curvature, that is, the radius of the droplet that encapsulates the colloidal mixture. The depth of the attractive potential between the PS particles and droplet interface is the sum of the depletion attraction, electrostatic repulsion, and steric repulsion from surfactant molecules. Without more information on these shortrange repulsive forces, we cannot estimate the well depth, but from the phase behavior and time scales for particles to dissociate from the interface, we estimate the well depth to be U m > 10k B T. 6.2 Equilibrium between bulk and surface In our analysis, we have assumed that the crystallization is a quasi2d process occurring from a 2D gas phase to a 2D solid phase confined to the wateroil droplet interfaces, with very little direct exchange of particles between the crystallites and the 3D interior of the droplet. This assumption is justified if practically all particles attach to the droplet interface, leaving very few particles in the interior. Particles confined to the interface lower their energy because of the depletion interaction between each particle and the surface, but have a lower entropy because they do not access the entire 3D volume of the droplet. The balance between entropy and energy determines the ratio of the number m of particles in the droplet interior to the number n at the surface, at equilibrium. This ratio is approximately m n V int V surf e ε/k BT 1 R 3 δ eε/k BT, (10) 11
26 where V int is the volume explored by the particles in the interior and V surf the volume explored by particles bound to the surface. These are set by the droplet radius R and the range of the interaction δ between the particles and the interface. Our experimental results for the spring constant k (see 6.6) suggest that the width of the potential well experienced by particles at the interface is δ 10 nm. The strength of the interaction between particles and the interface is ε/k B T 10. Hence m/n varies from about for the smallest experimental droplets with 5 µm radius to about 0.08 for the largest droplets with 50 µm radius. Even for the largest droplets, only a small fraction (less than 10%) of the colloidal particles remain in the bulk, and our treatment of crystallization as a quasi2d process is justified. Note that the attractive interactions between particles will reduce the number of particles in the bulk even more, because the particles at the interface further reduce their net free energy by forming stable crystallites. We do not observe stable crystallites in the interior volume of any of the droplets D phase behavior To calculate the phase diagram shown in Fig. S1, we first modeled the expected phase behavior for a flat 2D system in the absence of Gaussian curvature. We consider colloidal particles interacting through the potential described in Eq. 8. Given the short range of the attraction, 0.08 of the particle diameter, we expect any liquidgas coexistence region to be metastable and the equilibrium phase diagram to contain a single fluidsolid coexistence region (42 44). Although hexatic phases can also appear in such systems (45), we consider only fluid and solid phases, as these are the observed phases in the experimental system. The resulting phase diagram will allow us to clarify what we mean by rigid versus compliant coexisting crystals. Although the shortrange nature of the attractive part of the potential suppresses a triple point, we show that the rigid crystals studied here correspond to a sublimationlike region of the phase diagram. We consider a simple, firstorder model for the phase behavior. We use an equation of state for hard disks to model the fluid phase, and an Einstein solid model for the crystalline phase. These models provide analytical expressions for the free energies of both phases. To determine the phase diagram we evaluate the Helmholtz free energy per particle of both phases as a function of temperature and particle number density ρ. Phase coexistence is determined by equating the chemical potentials derived from these free energies. One unusual feature of our system is the temperaturedependence of the poly(nipam) depletant particles, which shrink as the temperature increases, changing both a s as well as the depletant volume fraction φ s in Eq. 8. Thus both the range and depth of the interaction potential decrease with temperature, and we expect the width of the coexistence region to decrease as well. To quantify this effect, we extract an empirical form for the depletant radius as a function of temperature a s (T ) by fitting a polynomial to the radius measured from dynamical light scattering (Fig. SM7). Assuming that no depletant molecules enter or leave the droplet as the temperature changes, we can calculate the temperaturedependent depletant volume fraction φ s (T ) = 0.25(a s (T )/a s (23 C)) 3 from this empirical relation, using an estimated volume fraction φ s = 0.25 at 23 C. We use these empirical relations to calculate the temperaturedependent pair potential in our model Fluid phase Because the shortranged attraction and screened electrostatic repulsion should not significantly affect the free energy of the fluid phase at the low densities observed in the experimental system, 12
27 42 40 Data y = (x 10) (x 10) ap/nm T/ C Fig. SM7. Variation of poly(nipam) depletant radius with temperature. The polynomial fit (green line) provides an empirical functional dependence a(t ) in the range 10 < T / C < 40, allowing us to calculate the phase diagram as a function of temperature. we model the fluid phase as a gas of hard disks of diameter d. The pair potential is {, r d v(r) = 0, r > d (11) The free energy of the fluid phase is calculated using an approximate equation of state for the hard disk fluid in two dimensions. This is expressed in terms of the compressibility factor Z β p/ρ = πβ pd 2 /(4η), with p the 2D pressure, ρ = N/V the number density corresponding to N particles in a volume V, η = πρd 2 /4 the area fraction and β = 1/k B T. For the harddisk system, close packing corresponds to η cp = π/(2 3) We use the Santosde HaroYuste approximate equation of state (46), Z(η) = [ ] 1 2η + 2η 1 cp 1 ηcp 2 η 2, (12) which is a good approximation over a wide range of particle densities, matching the first virial coefficient exactly and also reproducing the pole in the compressibility at close packing. The Helmholtz free energy F can be obtained by integrating the equation of state under constant temperature and particle number from the infinitely dilute system, which is the 2D ideal gas (ρ 0, F F ideal = Nk B T (log(ρλ 2 ) 1) where Λ = h/ 2πmk B T is the thermal de Broglie wavelength): F = F ideal + Nk B T ( 4ηΛ 2 β f βf N = log πd 2 ρ 0 ) 1 + Z(ρ) 1 dρ ; ρ η 0 Z(η) 1 dη, η (13) where we define f F/N. The chemical potential, or the Gibbs free energy per particle, can be expressed in terms of the compressibility factor Z: µ = G N = F + pv ; N β µ = β f + Z(η). (14) 13
28 6.3.2 Solid phase To model the chemical potential of the solid phase, we use the Einstein solid approximation, from which exact expressions of the free energy and entropy are easily obtained. We assume each colloidal particle sits in the minimum of the depletion potential well generated by six neighbors, arranged in a triangular lattice, and oscillates independently of these neighbors. Thus the 2D colloidal crystal can be treated as a collection of N independent harmonic oscillators with frequency ω = 3k/m (where k is the spring constant associated with small displacements about the minimum of the pairwise interaction U(r), and m is the mass of the particle) and depth ε 0 = 3U m. This approximation neglects the correlated fluctuations (phonons) of the solid, the fluctuations of particles normal to the interface, and the anharmonicity of the true potential. Such effects should produce only minor changes in the qualitative phase diagram calculated here. The partition function of the crystal is then Q N ω, where Q ω = e βε 0/(1 e β hω ) 2 is the partition function of a quantum harmonic oscillator with two degrees of freedom. The harmonic oscillator decouples in the z and y directions, and we ignore the zeropoint energy, which is minuscule compared to the well depth. Hence the Helmholtz free energy is βf = log(q N ω) Nβε 0 + 2N log(β hω), for β hω 1. (15) For the Einstein solid, volume is not an independent variable, and the chemical potential can be calculated from the Helmholtz free energy: ( ) ( ) F F β µ = β = β = βε 0 + 2log(β hω). (16) N V,T N T We rewrite this in terms of the thermal de Broglie wavelength for comparison with the fluid phase: β hω = Λ 3kd 2 d 2πk B T ( ) ( ) (17) Λ 2 3kd 2 β µ = βε 0 + log d 2 + log. 2πk B T Phase diagram Using approximate values for the spring constant and well depth from the theoretical pair potential, (section 6.1), we now equate the chemical potentials of the solid (Eq. 17) and fluid (Eq. 14) to determine the phase boundaries (note that the thermal de Broglie contributions cancel). Using Eq. 12 for the compressibility, we obtain η f (ρ f d 2 = 0.12) for the lowdensity boundary of the coexistence region at low temperature, when the depletant is at its maximum size. The density of the coexisting solid phase is very close to the closepacking density η s 0.9, as we have assumed a hexagonal Einstein solid with the particles at the minima of the depletion interaction, which gives rise to an interparticle distance of 1.02d. The low density of the fluid phase is in qualitative agreement with the experiments, where nearly all particles are observed to be in the solid phase at low temperature. Using other approximations for the hard disk equation of state in place of Eq. 12, such as the approximations in refs. (47) and (48), do not significantly change the results of this approximate theory. As the temperature increases, the coexistence region shrinks due to the change in depletant size, as shown in Fig. S1. Again, this is in qualitative agreement with experiments, which show that the system sublimates as the temperature increases. 14
29 In this phase diagram, we have assumed that the density of the solid phase remains that of a hexagonal lattice with lattice constant equal to the position of the minimum in the depletion potential, which depends weakly on a s. However, the stable solid phase at high temperature, when the depletion interaction is weak and even more shortranged, may be stabilized by entropy rather than the depletion attraction. For reference, computer simulations of the melting transition (49) of the pure harddisk system (with no attractions) show that there is coexistence between a fluid and entropic crystal between η f = (ρ f = 0.887/d 2 ) and η s = (ρ s = 0.904/d 2 ). Thus at temperatures greater than about 35 C, there could exist a coexistence between two solid phases, a dense crystal with η s 0.9 and an entropic crystal with η s 0.7 (43), but we have not modeled the equilibrium between solid phases in the phase diagram shown in Fig. S1. We note in passing that three different simulation methods have recently revealed a firstorder liquidhexatic transition in the highdensity regime for hard disks (50) Rigidity of the solid phase At temperatures below the volume phase transition of the poly(nipam) depletant particles where the depletion force has its maximum depth, and the coexistence region is broad we expect the crystals that form to be rigid due to the short range of the depletion potential. For a hexagonal network of springs of spring constant k, the the Lamé elastic constants are λ = µ = 3k/4 (51). At low temperature, the effective spring constant for our crystals is on the order of k B T /µm 2 (section 6.6). Thus the elastic constants are large (see section 6.4.2), and the crystal is rigid. The KosterlitzThouless parameter, 4µ(µ + λ) b 2 K = 2µ + λ k B T, (18) where the Burgers vector b d, is many orders of magnitude larger than 16π, the value at which the solid becomes stable against the formation of dislocations. The melting transition to an intermediate hexatic phase is therefore suppressed in favor of a sublimation directly into the fluid phase. At higher temperature, the crystal should become less rigid because the spring constant decreases as the depletants shrink. A compliant solid may exist at high temperature if an entropic crystal is favored over a crystal formed by depletion bonds. See ref. (50) for a progress report on understanding the phase behavior in this harddisklike regime Metastable fluidfluid coexistence Finally, we calculate the fluidfluid coexistence curve. Although the short range of attractions in the system makes any fluidfluid coexistence metastable relative to the fluidsolid phase separation identified in Section 6.3.3, the position of the fluidfluid coexistence curve can affect the kinetics of phase separation. Close to a fluidfluid critical point or in a region of fluidfluid coexistence, crystal growth may occur via a twostep nucleation mechanism (52, 53), where the dilute gas densifies into a dense droplet, within which the solid phase nucleates. To estimate whether such mechanisms are relevant in the experiments, we calculate the metastable fluidfluid coexistence curve in the 2D phase diagram, again in the absence of Gaussian curvature. To do so, we must include the effect of attraction between particles in the fluid phase, since there is no fluidfluid phase separation in the 2D harddisk fluid. To improve upon our approximate calculations in Section 6.3.1, we include the correction due to the attractive interactions to lowest order using perturbation theory (54). The reference system for our perturbation theory is the 2D harddisk fluid, with Helmholtz free energy per particle f ref given by Eq. 13. The approximate free 15
30 0.4 F F S S kb T U m Coexistence at 22 o C 0.1 F F Fig. SM8. Approximate phase diagram of a 2D system of particles experiencing a fixed pair potential set by the size and volume fraction of depletant at 22 C. In addition to the fluidsolid coexistence region, there is a metastable fluidfluid coexistence region indicated by the dotted curve. The dashed horizontal line shows the temperature at which crystallization takes place in the experiments. Η energy including the perturbative correction is (54) β f β f ref + ρ drg ref (r)[βu int (r)] (19) 2 where g ref is the radial distribution function of the hard disk reference system, and u int (r) is the perturbation potential which we take to be the attractive part of U(r). In our calculations, we use a density expansion to order ρ 3 for g ref (r), { 0, r < d g ref (r) 1 + ρg 1 (r) + ρ 2 g 2 (r) + ρ 3 (20) g 3 (r), r d where the g i (r) are numerically interpolated from the discrete values reported in Ref. (55). Using Eqs. 13 and 20 in Eq. 19, we obtain the Helmholtz free energy per particle in the fluid phase. The chemical potential, or the Gibbs free energy per particle, is: µ(η) = F + pv N = (η f ) η. (21) Fluidfluid coexistence occurs when the theoretical free energy first becomes concave. The coexistence densities are obtained by the usual Maxwell doubletangent construction. Including the perturbative effect of interactions in the fluid free energy does not significantly change the fluidsolid coexistence curves, justifying the use of the 2D harddisk fluid free energy to calculate Fig. S1. Significantly, our model does not show fluidfluid coexistence for interaction potentials corresponding to the experimentally accessible poly(nipam) depletant radius shown in Fig. SM7. A second fluid phase (signalled by µ/ η taking on negative values for some range of η) exists only when a s > 54 nm, larger than the maximal temperaturedependent poly(nipam) radius 16
31 in the experimental system. According to our model, the interactions at the maximal poly(nipam) radius of 40.7 nm are not strong enough even for a metastable fluidfluid coexistence. Every temperature value in Fig. S1 is associated with a unique interaction potential. To gauge the effect of possible metastable phases on crystal nucleation, we also calculate the theoretical phase diagram for the specific interaction potential at which the experiments are conducted, which corresponds to U(r) calculated using a s and φ s at the crystallization temperature of 22 C. As shown in Fig. SM8, crystallization in our experiments occurs far above the fluidfluid coexistence region (T /T c 3.2 1, where T c is the temperature of the fluidfluid critical point). Therefore, the effect of the metastable phases on the crystallization pathway is expected to be small Influence of curvature on the theoretical phase diagrams In our model, the primary effect of the curvature is to strain the crystal. We capture the effect of this strain on the free energy by adding an elastic energy penalty that depends on the shape of the solid domain, the curvature, and the effective spring constant of the pairwise interactions between particles. Here we show that we can neglect the effects of curvature on the interactions and the entropic contributions to the free energy. Because of the small size of the depletant, there is no direct influence of the droplet interface, and therefore of its curvature, on the pairwise depletion attractions. Furthermore, there should be no significant threebody contribution to the particleparticle interactions. The AsakuraOosawa interaction arises due to the overlap of regions from which the depletant is sterically excluded. The overlap of excluded volumes of two colloidal particles extends to at most a 2 s + 2a l a s = 0.20 µm for 2a l = 1.0 µm particles and 0.16 µm for 2a l = 0.6 µm particles, and does not overlap with the excluded volume near the droplet interface in either case. Threebody interactions occur only if the excluded volumes of three particles mutually overlap; the smallest depletant radius for which this happens is a l (2/ 3 1) = µm for 1.0 µm particles and µm for 0.6 µm particles, larger than the radius of the depletant in our system. Furthermore, the curvatureinduced strain is not large enough to cause threebody overlaps. The maximum curvatureinduced strain in the solid domains, as estimated from the domain widths, is of order (w/r)/ , smaller than the ratio of the potential well width to particle size, which is of order The entropic contribution to the free energy of the fluid phase, modeled using the harddisk fluid, is also not significantly modified by confining the disks to the surface of a sphere (56) (this is in contrast to surfaces of constant negative curvature, such as the hyperbolic surface, on which the behaviour of simple fluids can differ significantly from the flat plane (56).) A scaled particle theory approximation of the compressibility factor Z(η) for hard disks on the surface of a sphere (57) shows deviations of less than 1% for η 0.5 when the sphere radius is five times the particle diameter. For spheres with radii ten times the particle diameter, the deviations are less than 0.1%. 6.4 Nucleation and growth on curved surfaces In this section we show how we calculate the free energy of crystal growing on the surface of the sphere, as shown in Fig. 3 of the main text Classical theory of crystallization In classical nucleation theory (CNT), the free energy change of crystallization includes interfacial energy and bulk energy. The free energy change of creating a 2D crystallite of area A and interfacial length L is G = γ L f A, (22) 17
32 where γ is the interfacial tension associated with creating a solidgas interface of unit length, and f > 0 is the excess chemical potential per unit area in the gas phase compared to the solid phase. For a 2D circular disk of diameter a, L = πa and A = πa 2 /4. Rough estimates of γ and f can be obtained from the pair potential between individual particles, characterized by a well depth U m and equilibrium separation d. For our experimental system, d can be taken to be the diameter of the PS particles, since the depletion interaction is shortranged. The interfacial tension is estimated by considering the energy cost for a solid domain to break enough bonds to form a free boundary per unit length along the solidfluid interface. It corresponds to a particle breaking one bond (U m ) over a length of one particle size (d) along the interface. This gives the estimate of interfacial tension as: γ U m /d. (23) The free energy change between solid and gas phases per unit area is estimated from the chemical potential (the free energy per particle) in the solid phase. Each particle in the interior of the solid phase occupies the area of a regular hexagon with side d/ 3. From the Einstein solid estimate of the chemical potential in the solid phase, Eq. 17, we estimate f to be f 2 3 U m d 2 2 k B T 3 d 2 log ( 3kd 2 2πk B T ). (24) This estimate ignores entropic contributions from the fluid phase (aside from the trivial cancellation of the thermal de Broglie contribution), which depends on the the density of particles during crystallization. In the early stages of growth, when most particles are in the fluid phase and the fluid density is moderate, the entropic contribution is small and f remains positive (i.e. solidification is favoured) due to the dominant contribution of the depletion attraction in the solid phase (Eq. 24). However, as crystallization proceeds, the number of fluid particles and hence the fluid density becomes lower, increasing the entropic contribution to the gas phase free energy and decreasing f. At very low fluid densities (η 1), the entropic contribution dominates the contribution from Eq. 24, which is no longer accurate; f can even be zero or negative. Therefore, our rough estimate of the free energy change is valid only in the initial stages of growth. Growth stops when f 0, or when there are no particles left in the fluid phase Elastic energy of deformation On a flat surface, the PS particles can assemble in a perfect hexagonal lattice, with all bonds between particles at the equilibrium length of the depletion interaction. However, on a surface of nonzero Gaussian curvature, such as a sphere, geometry dictates that the lengths of all the bonds cannot be preserved, and they must undergo distortions from their equilibrium positions. To calculate the energy cost of changing bond lengths, we approximate each bond as a harmonic potential with spring constant k and with equilibrium bond length the same as that of the depletion interaction. In the continuum limit where the bond lengths are small compared to the size of the bond network, the deformation energy of the hexagonal network is equivalent to the elastic energy of deforming a twodimensional membrane with a 2D Young s modulus Y and Poisson ratio ν given by (51): Y = 2 3 k; ν = 1 3. (25) Within this continuum description, the elastic energy of a membrane is given in terms of the 2 2 strain tensor u i j (58): E s = 1 d 2 Y [ r (u11 2 2(1 ν 2 + u 22 ) 2 2(1 ν)(u 11 u 22 u 2 ) 12) ], (26) 18
33 where the integral is over the surface of the undeformed patch. To find the elastic energy of deforming a membrane patch of a particular shape on a sphere of radius R, we must solve the variational problem of finding the strain fields that minimize the elastic energy, subject to the boundary conditions of zero line stresses perpendicular to the boundaries, so that the displacements of the patch bring it to the required spherical shape. This is a difficult problem to solve for patches of arbitrary shape, but it has been solved for some specific shapes. For discshaped elastic domains of diameter a, the elastic energy cost (23) is: E disc π ( Y a ) 6 R2. (27) R For rectangular domains with length l much larger than width w, an approximate expression for the elastic deformation energy on a sphere (27) is: E ribbon = 1 640(1 ν 2 ) Y R2 ( w 5 ) l R Y R2 ( w 5 ) l R 6 for ν = 1/3. We use Eq. 27 and Eq. 28 to estimate the elastic energy cost of stretching a solid domain on the curved surface in the main text. (28) 6.5 Kinetic growth instability calculations In the main text we rule out kinetic instabilities as a cause of the observed anisotropic crystal shapes by comparing growth on curved and flat substrates and estimating the relevant physical parameters. Here we describe the details of this calculation. Growth instabilities arise when diffusion of the fluid particles to the crystalfluid interface is the ratelimiting step in crystal growth, which is true for large crystals. Since it takes fluid particles longer to diffuse around the interface for larger crystals, smoothing out protuberances in the growing interface may be kinetically prohibited for large crystals even if energetically favored. This leads to a dendritic growth instability for crystallites larger than a certain size. Our flat crystals, which are up to 40 µm in diameter, do not exhibit dendritic growth. Since the growth conditions and particle concentrations are similar in our experiments on flat and curved substrates, we do not expect dendritic growth to be observed up to these sizes on curved substrates either. This argument can be made quantitative by estimating the characteristic crystal size at which growth instabilities become important. A simple physical model for growth instabilities leading to dendrites is the linear stability analysis of Mullins and Sekerka (4, 21, 22). A flat crystalfluid interface growing into the fluid phase is expected to be unstable to perturbations of wavelength longer than the MullinsSekerka wavelength λ s = 2π l d l c /2, (29) where l d is the macroscopic diffusion length and l c is the microscopic capillary length. l d = 2D/v for fluid particles with diffusion constant D diffusing to an interface growing at speed v. l c depends on the energy of the solidliquid interface: l c = γ ( c) 2 ( f / c), (30) where γ is the line tension of the crystalfluid interface, c is the jump in concentration c between the two phases, and f is the chemical potential. The capillary length is difficult to calculate or measure directly, but it is essentially the interfacial thickness (4), which is at least one particle diameter in our 19
34 system. Choosing l c = d to find the lower bound on the MullinsSekerka wavelength, and estimating the interfacial growth speed from our experiments, we obtain λ s 100 µm on planar substrates for both 0.6µm and 1.0µmdiameter particles. This is the characteristic width of dendrites if a kinetic instability is responsible for anisotropic growth. Crystals that are smaller than λ s will not show a dendritic instability, consistent with our observations on flat crystals. Because the diffusion length l d and capillary length l c do not depend strongly on the substrate curvature, the MullinsSekerka wavelength λ s should not change significantly when the crystal grows on a curved surfaces. In fact, λ s is likely to be larger for a curved surface because of two effects. First, the free energy change associated with crystallization is smaller on a curved surface, because of the positive elastic energy cost associated with crystal growth. Thus the capillary length l c should be larger on a curved surface. Second, for crystals of the same diameter, the fluid particles have a smaller interfacial length to explore since the perimeter is smaller on a curved surface compared to a flat surface. The diffusion of fluid particles to interfacial irregularities is faster, which helps to stabilize the interface. As a result, we do not expect the dendritic instability to appear on curved surfaces if the crystal sizes are smaller than 100 µm, which we consider a lower bound on the dendrite width. Our characteristic width of anisotropic growth is much smaller, even for our largest droplets: the biggest domain width is about 20 µm for 1.0µm PS particles, and 25 µm for 0.6µm PS particles. Thus we rule out a dendritic growth instability as the mechanism for anisotropic growth in our curved crystals. 6.6 Estimation of spring constant As we discuss in the main text, we are able to fit the model to the observed domain widths to extract an effective spring constant for the interparticle interactions. This section describes our method. Our theoretical model predicts a constant width w for an anisotropic crystallite grown on a curved surface. The stable domain width can be determined from our model by minimizing the net free energy of forming a ribbonlike domain as a function of domain width w: w 4 ( ) 2 f 1/4 R. (31) 3 Y where we have used rough estimates of f and Y based on the well depth U m and spring constant k of the interparticle pair potential (Eq. 24 and Eq. 25). While we expect the well depth to be reasonably close to U m = 4k B T for 1.0 µm PS particles and U m = 2.5k B T for 0.6 µm particles, the theoretical estimate of the spring constant is less reliable, since it depends on the details of the shortranged repulsive interactions between particles. However, we can estimate k from the dependence of the domain width on droplet radius observed in the experiments. Using a linear regression in Fig. S4B, we extract a slope of 0.10 for the w /dvs.r/d relationship for domains of d = 0.6 µm particles, and a slope of 0.17 for domains of d = 1.0 µm particles. Using Eq. 31, we estimate the spring constant as k k B T /µm 2 for 0.6 µm particles and k k B T /µm 2 for 1.0 µm particles. The spring constant estimate for 1.0 µm PS particles is consistent with the estimate of k B T /µm 2 from the theoretical pair potential, Eq. 8. The value of 10 5 k B T /µm 2 for the spring constant is also consistent with that obtained from measurements of the ensemble probability of certain types of nonrigid clusters of 1.0 µm PS particles under a similar depletion attraction potential (35). As discussed in ref. (35), the probability of observing a nonrigid clusters relative to all other clusters, including rigid and other nonrigid structures, depends on the spring constant of the potential through the vibrational entropy of the soft mode. The experimentally measured probability of a 9particle nonrigid cluster of 1.0 µm particles 20
35 30 Probability (\%) k (kb T/µm2) Fig. SM9. Theoretical equilibrium probability of observing a nonrigid cluster of 9 particles as a function of spring constant. The computer rendering shows the structure of the nonrigid cluster. The equilibrium probability (the black solid line) depends on the spring constant k and is independent of the potential well depth. Black dots shows the region of 95% confidence interval of the experimental measurement of the equilibrium probability of observing the nonrigid cluster. was 11%, lying between 4% and 27% with a 95% confidence interval. The actual pair potential between PS particles can be approximated by a harmonic potential 1 U( r) = k r2 Um, 2 (32) where Um is the strength of the potential, r is the distance between particles around the equilibrium position, and k is the spring constant. Using a statistical mechanical model to predict the probabilities of all other clusters (35 ) and a numerical calculation of the vibrational entropy associated with the soft mode (see Supplemental Information in ref. (35 )), we can estimate the theoretical probability of observing the nonrigid cluster Ptheory. Because the number of bonds is the same for all clusters, Ptheory depends only on the spring constant k and is independent from the well depth Um. Fig. SM9 shows how Ptheory varies with the spring constant k. The range Ptheory =4% 27% corresponds to spring constants between kb T /µm2 and kb T /µm2 for 1.0 µm PS particles. 21
Randomly Triangulated Surfaces as Models for Fluid and Crystalline Membranes. G. Gompper Institut für Festkörperforschung, Forschungszentrum Jülich
Randomly Triangulated Surfaces as Models for Fluid and Crystalline Membranes G. Gompper Institut für Festkörperforschung, Forschungszentrum Jülich Motivation: Endo and Exocytosis Membrane transport of
More informationColloidal Particles at Liquid Interfaces: An Introduction
1 Colloidal Particles at Liquid Interfaces: An Introduction Bernard P. Binks and Tommy S. Horozov Surfactant and Colloid Group, Department of Chemistry, University of Hull, Hull, HU6 7RX, UK 1.1 Some Basic
More informationSupporting Information
Supporting Information Visible LightDriven BiOIBased Janus Micromotors in Pure Water Renfeng Dong, a Yan Hu, b Yefei Wu, b Wei Gao, c Biye Ren, b* Qinglong Wang, a Yuepeng Cai a* a School of Chemistry
More informationChapter 10. Lesson Starter. Why did you not smell the odor of the vapor immediately? Explain this event in terms of the motion of molecules.
Preview Lesson Starter Objectives The KineticMolecular Theory of Gases The KineticMolecular Theory and the Nature of Gases Deviations of Real Gases from Ideal Behavior Section 1 The KineticMolecular
More informationInterfacial forces and friction on the nanometer scale: A tutorial
Interfacial forces and friction on the nanometer scale: A tutorial M. Ruths Department of Chemistry University of Massachusetts Lowell Presented at the Nanotribology Tutorial/Panel Session, STLE/ASME International
More informationPhysics and Chemistry of Interfaces
Hans Jürgen Butt, Karlheinz Graf, and Michael Kappl Physics and Chemistry of Interfaces Second, Revised and Enlarged Edition WILEY VCH WILEYVCH Verlag GmbH & Co. KGaA Contents Preface XI 1 Introduction
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationINTERMOLECULAR AND SURFACE FORCES
INTERMOLECULAR AND SURFACE FORCES SECOND EDITION JACOB N. ISRAELACHVILI Department of Chemical & Nuclear Engineering and Materials Department University of California, Santa Barbara California, USA ACADEMIC
More informationFluidsolid transitions on walls in binary hardsphere mixtures
EUROPHYSICS LETTERS 1 November 1997 Europhys. Lett., 40 (3), pp. 337342 (1997) Fluidsolid transitions on walls in binary hardsphere mixtures A. D. Dinsmore 1,P.B.Warren 2,W.C.K.Poon 3 and A. G. Yodh
More informationThe FreeEnergy Landscape of Clusters of Attractive Hard Spheres
The FreeEnergy Landscape of Clusters of Attractive Hard Spheres The Harvard community has made this article openly available. Please share how this access benefits you. Your story matters. Citation Published
More informationFrom Polymer Gel Nanoparticles to Nanostructured Bulk Gels
From Polymer Gel Nanoparticles to Nanostructured Bulk Gels Zhibing Hu Departments of Physics and Chemistry, University of North Texas Denton, TX 76203, U. S. A. Phone: 940565 4583, FAX: 9405654824,
More informationChapter 10: Liquids, Solids, and Phase Changes
Chapter 10: Liquids, Solids, and Phase Changes Inchapter exercises: 10.1 10.6, 10.11; Endofchapter Problems: 10.26, 10.31, 10.32, 10.33, 10.34, 10.35, 10.36, 10.39, 10.40, 10.42, 10.44, 10.45, 10.66,
More informationLiquid crystal phase transitions in dispersions of rodlike colloidal particles
J. Phys.: Condens. Matter 8 (1996) 9451 9456. Printed in the UK Liquid crystal phase transitions in dispersions of rodlike colloidal particles M P B van Bruggen, F M van der Kooij and HNWLekkerkerker
More informationDescription: Supplementary Figures, Supplementary Methods, and Supplementary References
File Name: Supplementary Information Description: Supplementary Figures, Supplementary Methods, and Supplementary References File Name: Supplementary Movie 1 Description: Footage of time trace of seeds
More informationColloidal Suspension Rheology Chapter 1 Study Questions
Colloidal Suspension Rheology Chapter 1 Study Questions 1. What forces act on a single colloidal particle suspended in a flowing fluid? Discuss the dependence of these forces on particle radius. 2. What
More informationSupporting Information
Supporting Information Janus Hollow Spheres by Emulsion Interfacial SelfAssembled SolGel Process Fuxin Liang, Jiguang Liu, Chengliang Zhang, Xiaozhong Qu, Jiaoli Li, Zhenzhong Yang* State Key Laboratory
More informationSwelling and Collapse of Single Polymer Molecules and Gels.
Swelling and Collapse of Single Polymer Molecules and Gels. CoilGlobule Transition in Single Polymer Molecules. the coilglobule transition If polymer chains are not ideal, interactions of nonneighboring
More informationStates of matter. Chapter 11. Kinetic Molecular Theory of Liquids and Solids. Kinetic Molecular Theory of Solids Intermolecular Forces
States of matter Chapter 11 Intermolecular Forces Liquids and Solids By changing the T and P, any matter can exist as solid, liquid or gas. Forces of attraction determine physical state Phase homogeneous
More informationSupplementary Figure 1 Experimental setup for crystal growth. Schematic drawing of the experimental setup for C 8 BTBT crystal growth.
Supplementary Figure 1 Experimental setup for crystal growth. Schematic drawing of the experimental setup for C 8 BTBT crystal growth. Supplementary Figure 2 AFM study of the C 8 BTBT crystal growth
More informationThey are similar to each other
They are similar to each other Different than gases. They are incompressible. Their density doesn t change much with temperature. These similarities are due to the molecules staying close together in solids
More informationSurfactantfree exfoliation of graphite in aqueous solutions
Surfactantfree exfoliation of graphite in aqueous solutions Karen B. Ricardo, Anne Sendecki, and Haitao Liu * Department of Chemistry, University of Pittsburgh, Pittsburgh, PA 15260, U.S.A 1. Materials
More informationSolids / Crystal Structure
The first crystal analysis proved that in the typical inorganic salt, NaCl, there is no molecular grouping. The inference that the structure consists of alternate ions of sodium and chlorine was an obvious
More informationSupporting Information
Supporting Information PhenylModified Carbon Nitride Quantum Dots with Distinct Photoluminescence Behavior Qianling Cui, Jingsan Xu,* Xiaoyu Wang, Lidong Li,* Markus Antonietti, and Menny Shalom anie_201511217_sm_miscellaneous_information.pdf
More informationThe first three categories are considered a bottomup approach while lithography is a topdown
Nanowires and Nanorods Onedimensional structures have been called in different ways: nanowires, nanorod, fibers of fibrils, whiskers, etc. The common characteristic of these structures is that all they
More informationSUPPLEMENTARY INFORMATION
Actuation of shapememory colloidal fibres of Janus ellipsoids Aayush A. Shah, 1# Benjamin Schultz, 2# Wenjia Zhang, 3 Sharon C. Glotzer 1,2,3 and Michael J. Solomon 1,3* 1 Macromolecular Science and Engineering,
More informationThey are similar to each other. Intermolecular forces
s and solids They are similar to each other Different than gases. They are incompressible. Their density doesn t change much with temperature. These similarities are due to the molecules staying close
More informationHolographic Characterization of Agglomerates in CMP Slurries
Holographic Characterization of Agglomerates in CMP Slurries Total Holographic Characterization (THC) Comparison of THC to other technologies Dynamic Light Scattering (DLS) Scanning Electron Microscopy
More informationAmorphous Polymers: Polymer Conformation Laboratory 1: Module 1
D E P A R T M E N T O F M A T E R I A L S S C I E N C E A N D E N G I N E E R I N G M A S S A C H U S E T T S I N S T I T U T E O F T E C H N O L O G Y 3.014 Materials Laboratory Fall 2008 Amorphous Polymers:
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationChapter 10. Liquids and Solids
Chapter 10 Liquids and Solids Section 10.1 Intermolecular Forces Section 10.1 Intermolecular Forces Section 10.1 Intermolecular Forces Section 10.1 Intermolecular Forces Metallic bonds Covalent bonds Ionic
More informationBasic Laboratory. Materials Science and Engineering. Atomic Force Microscopy (AFM)
Basic Laboratory Materials Science and Engineering Atomic Force Microscopy (AFM) M108 Stand: 20.10.2015 Aim: Presentation of an application of the AFM for studying surface morphology. Inhalt 1.Introduction...
More informationFigure 43. Some common mechanical systems involving contact.
33 Demonstration: experimental surface measurement ADE PhaseShift Whitelight Interferometer Surface measurement Surface characterization  Probability density function  Statistical analyses  Autocorrelation
More informationRapid Preparation of Polymersomes by a Water Addition/Solvent Evaporation Method. Supporting Information
Rapid Preparation of Polymersomes by a Water Addition/Solvent Evaporation Method Supporting Information Hana Robson Marsden, Luca Gabrielli, Alexander Kros* Department of Soft Matter Chemistry, Leiden
More informationLecture Presentation. Chapter 11. Liquids and Intermolecular Forces Pearson Education, Inc.
Lecture Presentation Chapter 11 Liquids and States of Matter The fundamental difference between states of matter is the strength of the intermolecular forces of attraction. Stronger forces bring molecules
More informationColloidal Crystal: emergence of long range order from colloidal fluid
Colloidal Crystal: emergence of long range order from colloidal fluid Lanfang Li December 19, 2008 Abstract Although emergence, or spontaneous symmetry breaking, has been a topic of discussion in physics
More informationObservation of sizeindependent effects in nanoparticle retention behavior during asymmetricflow fieldflow fractionation
Analytical and Bioanalytical Chemistry Electronic Supplementary Material Observation of sizeindependent effects in nanoparticle retention behavior during asymmetricflow fieldflow fractionation Julien
More informationConfocal Microscopy Imaging of Single Emitter Fluorescence and Hanbury Brown and Twiss Photon Antibunching Setup
1 Confocal Microscopy Imaging of Single Emitter Fluorescence and Hanbury Brown and Twiss Photon Antibunching Setup Abstract Jacob Begis The purpose of this lab was to prove that a source of light can be
More informationSupplementary Material (ESI) for Chemical Communications This journal is (c) The Royal Society of Chemistry 2009
1. Materials: Styrene (St), methyl methacrylate (MMA) and acrylic acid (AA) (Lingfeng Chemical reagent Co. Ltd, Shanghai, China) were distilled and stored at 4 ºC if not used immediately, ammonium persulfate
More informationAttractive interaction between likecharged repulsive particles at liquidliquid interfaces.
1 Attractive interaction between likecharged repulsive particles at liquidliquid interfaces. M.G. Nikolaides*,, A.R. Bausch*,, M.F. Hsu *, A.D. Dinsmore *, M.P. Brenner, C. Gay, and D.A. Weitz *,. *
More informationChapter 10: Liquids and Solids
Chapter 10: Liquids and Solids Chapter 10: Liquids and Solids *Liquids and solids show many similarities and are strikingly different from their gaseous state. 10.1 Intermolecular Forces Intermolecular
More informationChapter 11. Liquids and Intermolecular Forces
Chapter 11. Liquids and Intermolecular Forces 11.1 A Molecular Comparison of Gases, Liquids, and Solids Gases are highly compressible and assume the shape and volume of their container. Gas molecules are
More informationAtomic Force Microscopy imaging and beyond
Atomic Force Microscopy imaging and beyond Arif Mumtaz Magnetism and Magnetic Materials Group Department of Physics, QAU Coworkers: Prof. Dr. S.K.Hasanain M. Tariq Khan Alam Imaging and beyond Scanning
More informationSupporting Information. Near infrared lightpowered Janus mesoporous silica nanoparticle motors
Supporting Information Near infrared lightpowered Janus mesoporous silica nanoparticle motors Mingjun Xuan,, Zhiguang Wu,, Jingxin Shao, Luru Dai, Tieyan Si,, * and Qiang He, * State Key Laboratory of
More informationProteins in solution: chargetuning, cluster formation, liquidliquid phase separation, and crystallization
HERCULES Specialized Course: Nonatomic resolution scattering in biology and soft matter Grenoble, September 1419, 2014 Proteins in solution: chargetuning, cluster formation, liquidliquid phase separation,
More informationMonolayers. Factors affecting the adsorption from solution. Adsorption of amphiphilic molecules on solid support
Monolayers Adsorption as process Adsorption of gases on solids Adsorption of solutions on solids Factors affecting the adsorption from solution Adsorption of amphiphilic molecules on solid support Adsorption
More informationSelfAssembly. SelfAssembly of Colloids.
SelfAssembly Lecture 56 SelfAssembly of Colloids. Liquid crystallinity Colloidal Stability and Phases The range of forces attractive and repelling forces exists between the colloidal particles van der
More informationBRIEF COMMUNICATION TO SURFACES ANALYSIS OF ADHESION OF LARGE VESICLES
BRIEF COMMUNICATION ANALYSIS OF ADHESION OF LARGE VESICLES TO SURFACES EVAN A. EVANS, Department ofbiomedical Engineering, Duke University, Durham, North Carolina 27706 U.S.A. ABSTRACT An experimental
More informationHighly Controlled Synthesis and SuperRadiant. Photoluminescence of Plasmonic CubeinCube. Nanoparticles
Supporting Information Highly Controlled Synthesis and SuperRadiant Photoluminescence of Plasmonic CubeinCube Nanoparticles JeongEun Park, Sungi Kim, Jiwoong Son, Yeonhee Lee and JwaMin Nam* Department
More informationHybrid Gold Superstructures: Synthesis and. Specific Cell Surface Protein Imaging Applications
Supporting Information Hybrid Gold Nanocube@Silica@GrapheneQuantumDot Superstructures: Synthesis and Specific Cell Surface Protein Imaging Applications Liu Deng, Ling Liu, Chengzhou Zhu, Dan Li and Shaojun
More informationFilm Formation from Industrial Waterborne Latices
Film Formation from Industrial Waterborne Latices I. Ludwig*, W. Schabel*, J.C. Castaing**, P. Ferlin**, M. Kind* *Universität Karlsruhe (TH), Germany **Rhodia Recherches, Aubervilliers, France Abstract
More informationCHEMISTRY Matter and Change. Chapter 12: States of Matter
CHEMISTRY Matter and Change Chapter 12: States of Matter CHAPTER 12 States of Matter Section 12.1 Section 12.2 Section 12.3 Section 12.4 Gases Forces of Attraction Liquids and Solids Phase Changes Click
More informationThe Counter Rotating ConePlate Shear Cell
2 The Counter Rotating ConePlate Shear Cell Abstract We report on novel possibilities to study colloidal suspensions in a steady shear field in real space. Fluorescence confocal microscopy is combined
More informationarxiv:condmat/ v1 [condmat.other] 5 Jun 2004
arxiv:condmat/0406141v1 [condmat.other] 5 Jun 2004 Moving Beyond a Simple Model of Luminescence Rings in Quantum Well Structures D. Snoke 1, S. Denev 1, Y. Liu 1, S. Simon 2, R. Rapaport 2, G. Chen 2,
More informationName Class Date. How do mixtures differ from elements and compounds? How can mixtures be separated? What are solutions?
CHAPTER 3 3 Mixtures SECTION Elements, Compounds, and Mixtures BEFORE YOU READ After you read this section, you should be able to answer these questions: How do mixtures differ from elements and compounds?
More informationOnepot synthesis of micron partly hollow anisotropic dumbbell shaped silica coreshell particles
Electronic Supplementary Material (ESI) for ChemComm. This journal is The Royal Society of Chemistry 2016 Supporting Information Onepot synthesis of micron partly hollow anisotropic dumbbell shaped silica
More informationStation 1 Water is a polar molecule and has a very unique structure
Station 1 Water is a polar molecule and has a very unique structure A water molecule, because of its shape, is a polar molecule. That is, it has one side that is positively charged and one side that is
More informationLECTURE 4: Marangoni flows
LECTURE 4: Marangoni flows Marangoni flows are those driven by surface tension gradients. In general, surface tension σ depends on both the temperature and chemical composition at the interface; consequently,
More informationPHASE TRANSITIONS IN SOFT MATTER SYSTEMS
OUTLINE: Topic D. PHASE TRANSITIONS IN SOFT MATTER SYSTEMS Definition of a phase Classification of phase transitions Thermodynamics of mixing (gases, polymers, etc.) Meanfield approaches in the spirit
More informationThe new physiology of visionchapter The colours of interference. SIR C V RAMAN Received October 14, 1965
Proc. Indian Acad. Sci. A62 243248 (1965) The new physiology of visionchapter The colours of interference XXVII. SIR C V RAMAN Received October 14, 1965 The characteristic features and properties of
More informationPractical 1P9 Polymers  Molecular weight effects
Practical 1P9 Polymers  Molecular weight effects What you should learn from this practical Science The main theme of the Polymer Synthesis lectures is that molecular weight, and the ability to control
More informationSupporting Information Surface Tension Mediated Conversion of Light to Work
Supporting Information Surface Tension Mediated Conversion of Light to Work David Okawa, Stefan J. Pastine, Alex Zettl, and Jean M. J. Fréchet * College of Chemistry and Department of Physics, University
More informationPARTICLE SIZE ANALYSIS OF GOLD NANOPARTICLES
PARTICLE SIZE ANALYSIS OF GOLD NANOPARTICLES Scientific interest in well dispersed suspensions of colloidal gold (or nanoparticles) can be traced back to ancient times. Original uses of colloidal gold
More informationIonic Bonds. H He: ... Li Be B C :N :O :F: :Ne:
Ionic Bonds Valence electrons  the electrons in the highest occupied energy level  always electrons in the s and p orbitals  maximum of 8 valence electrons  elements in the same group have the same
More informationSupporting Information
Electronic Supplementary Material (ESI) for Analyst. This journal is The Royal Society of Chemistry 2015 Supporting Information Experimental Methods Instrumentation Zeta potentials and sizes of colloidal
More informationSynthesis and characterization of hybride polyaniline / polymethacrylic acid/ Fe 3 O 4 nanocomposites
Synthesis and characterization of hybride polyaniline / polymethacrylic acid/ Fe 3 O 4 nanocomposites Mohammad Reza Saboktakin*, Abel Maharramov, Mohammad Ali Ramazanov Department of Chemistry, Baku State
More informationSurface and Interfacial Tensions. Lecture 1
Surface and Interfacial Tensions Lecture 1 Surface tension is a pull Surfaces and Interfaces 1 Thermodynamics for Interfacial Systems Work must be done to increase surface area just as work must be done
More informationSUPPLEMENTARY INFORMATION
SUPPLEMENTARY INFORMATION doi: 1.138/nnano.21.29 Gammadion fabrication The gammadions were designed using CAD software with a line width of 8 nm and a periodicity of 8 nm, figure S1. They were arrayed
More informationPREPARATION AND CHARACTERISATION OF PERFLUORODECALIN IN WATER PICKERING EMULSION
PREPARATION AND CHARACTERISATION OF PERFLUORODECALIN IN WATER PICKERING EMULSION L.S. Chin, M.Lim, R.Amal 1 1 ARC Centre of Excellence for Functional Nanomaterial, School of Chemical Engineering, The University
More informationCHARACTERIZATION of NANOMATERIALS KHP
CHARACTERIZATION of NANOMATERIALS Overview of the most common nanocharacterization techniques MAIN CHARACTERIZATION TECHNIQUES: 1.Transmission Electron Microscope (TEM) 2. Scanning Electron Microscope
More informationMohamed Daoud Claudine E.Williams Editors. Soft Matter Physics. With 177 Figures, 16 of them in colour
Mohamed Daoud Claudine E.Williams Editors Soft Matter Physics With 177 Figures, 16 of them in colour Contents 1. Droplets: CapiUarity and Wetting 1 By F. BrochardWyart (With 35 figures) 1.1 Introduction
More informationGRAVIMETRIC ANALYSIS
GRAVIMETRIC ANALYSIS Gravimetric methods are quantitative methods in which the mass of the analyte or some compound that is chemically related to the analyte is determined. What are the steps in a gravimetric
More informationChapter 12. Insert picture from First page of chapter. Intermolecular Forces and the Physical Properties of Liquids and Solids
Chapter 12 Insert picture from First page of chapter Intermolecular Forces and the Physical Properties of Liquids and Solids Copyright McGrawHill 2009 1 12.1 Intermolecular Forces Intermolecular forces
More informationSynthesis of Copper Oxide Nanoparticles in Droplet Flow Reactors
University of New Hampshire University of New Hampshire Scholars' Repository Honors Theses and Capstones Student Scholarship Spring 2017 Synthesis of Copper Oxide Nanoparticles in Droplet Flow Reactors
More informationSelfassembled nanostructures for antireflection optical coatings
Selfassembled nanostructures for antireflection optical coatings Yang Zhao 1, Guangzhao Mao 2, and Jinsong Wang 1 1. Deaprtment of Electrical and Computer Engineering 2. Departmentof Chemical Engineering
More informationDynamic Self Assembly of Magnetic Colloids
Institute of Physics, University of Bayreuth Advanced Practical Course in Physics Dynamic Self Assembly of Magnetic Colloids A. Ray and Th. M. Fischer 3 2012 Contents 1. Abstract 3 2. Introduction 3 3.
More informationEE C247B / ME C218 INTRODUCTION TO MEMS DESIGN SPRING 2014 C. Nguyen PROBLEM SET #4
Issued: Wednesday, Mar. 5, 2014 PROBLEM SET #4 Due (at 9 a.m.): Tuesday Mar. 18, 2014, in the EE C247B HW box near 125 Cory. 1. Suppose you would like to fabricate the suspended cross beam structure below
More informationWater and Aqueous Systems
Water and Aqueous Systems The Water Molecule: a Review Water is a simple triatomic molecule, H 2 O Each OH bond is highly polar, because of the high electronegativity of the oxygen (N, O, F, and Cl have
More informationExperimental Colloids I (and I)
Experimental Colloids I (and I) Dave Weitz Harvard http://www.seas.harvard.edu/projects/weitzlab Boulder Summer School 7/24/17 Experimental Colloids I (and I) Dave Weitz Harvard http://www.seas.harvard.edu/projects/weitzlab
More informationRheology, Adhesion, and Debonding of Lightly Crosslinked Polymer Gels
Rheology, Adhesion, and Debonding of Lightly Crosslinked Polymer Gels Nicholas B. Wyatt, and Anne M. Grillet 2 Materials Science and Engineering Division 2 Engineering Sciences Division Sandia National
More informationSupplementary Information
Supplementary Information Facile preparation of superhydrophobic coating by spraying a fluorinated acrylic random copolymer micelle solution Hui Li, a,b Yunhui Zhao a and Xiaoyan Yuan* a a School of Materials
More informationVolume 7 Number 5 7 March 2011 Pages
www.rsc.org/softmatter Volume 7 Number 5 7 March 2011 Pages 1545 2164 ISSN 1744683X COMMUNICATION Stefano Sacanna et al. Lock and key colloids through polymerizationinduced buckling of monodisperse silicon
More informationProtein separation and characterization
Address:800 S Wineville Avenue, Ontario, CA 91761,USA Website:www.aladdine.com Email USA: tech@aladdine.com Email EU: eutech@aladdine.com Email Asia Pacific: cntech@aladdine.com Protein separation
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationDetailed AFM Force Spectroscopy of the Interaction between. CD44IgGFusion Protein and Hyaluronan
Electronic Supplementary Material to: Detailed AFM Force Spectroscopy of the Interaction between CD44IgGFusion Protein and Hyaluronan Aernout A. Martens a, Marcel Bus a, Peter C. Thüne b,, Tjerk H. Oosterkamp,
More informationLiquids and Intermolecular Forces. Course Learning Outcomes for Unit I. Reading Assignment. Unit Lesson UNIT I STUDY GUIDE
UNIT I STUDY GUIDE Liquids and Intermolecular Forces Course Learning Outcomes for Unit I Upon completion of this unit, students should be able to: 1. Identify the intermolecular attractive interactions
More informationNanoparticle Tracking Analysis; Sizing, Counting and Visualizing of Nanoparticles. Dr Bob Carr, Founder and CTO NanoSight Ltd
Nanoparticle Tracking Analysis; Sizing, Counting and Visualizing of Nanoparticles Dr Bob Carr, Founder and CTO NanoSight Ltd The Instrument Range See us at LM10 Series LM20 NS500 NanoSight s Technology
More informationSUPPLEMENTARY INFORMATION
SUPPLEMENTARY INFORMATION Covalent Bulk Functionalization of Graphene Jan M. Englert a, Christoph Dotzer a, Guang Yang b, Martin Schmid c, Christian Papp c, J. Michael Gottfried c, HansPeter Steinrück
More information21 The Nature of Matter. Atoms
21 The Nature of Matter Atoms What do we call the smallest unit of matter? Who named it? What does it mean in Greek? How many atoms would make a row 1cm long? What does this indicate? Atoms are made up
More informationThicknessinduced morphology changes in lamellar diblock copolymer ultrathin films
EUROPHYSICS LETTERS 15 December 1997 Europhys. Lett., 40 (6), pp. 643648 (1997) Thicknessinduced morphology changes in lamellar diblock copolymer ultrathin films T. L. Morkved and H. M. Jaeger The James
More informationMATERIALS SCIENCE POLYMERS
POLYMERS 1) Types of Polymer (a) Plastic Possibly the largest number of different polymeric materials come under the plastic classification. Polyethylene, polypropylene, polyvinyl chloride, polystyrene,
More informationSupplementary Information
Supplementary Information Timedependent growth of zinc hydroxide nanostrands and their crystal structure Xinsheng Peng, ab Jian Jin, a Noriko Kobayashi, a Wolfgang Schmitt, c and Izumi Ichinose* a a Organic
More information2. As gas P increases and/or T is lowered, intermolecular forces become significant, and deviations from ideal gas laws occur (van der Waal equation).
A. Introduction. (Section 11.1) CHAPTER 11: STATES OF MATTER, LIQUIDS AND SOLIDS 1. Gases are easily treated mathematically because molecules behave independently. 2. As gas P increases and/or T is lowered,
More informationIntermolecular Forces and Liquids and Solids. Chapter 11. Copyright The McGraw Hill Companies, Inc. Permission required for
Intermolecular Forces and Liquids and Solids Chapter 11 Copyright The McGraw Hill Companies, Inc. Permission required for 1 A phase is a homogeneous part of the system in contact with other parts of the
More informationSupporting Online Material for
www.sciencemag.org/cgi/content/full/323/5912/362/dc1 Supporting Online Material for Morphogenesis of SelfAssembled Nanocrystalline Materials of Barium Carbonate and Silica This PDF file includes: Juan
More informationSOLIDS AND LIQUIDS  Here's a brief review of the atomic picture or gases, liquids, and solids GASES
30 SOLIDS AND LIQUIDS  Here's a brief review of the atomic picture or gases, liquids, and solids GASES * Gas molecules are small compared to the space between them. * Gas molecules move in straight lines
More informationModel Worksheet Teacher Key
Introduction Despite the complexity of life on Earth, the most important large molecules found in all living things (biomolecules) can be classified into only four main categories: carbohydrates, lipids,
More informationElectronic Supplementary Information
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A. This journal is The Royal Society of Chemistry 2017 Electronic Supplementary Information A coaxial triboelectric nanogenerator
More informationSUPPLEMENTARY FIGURES
SUPPLEMENTARY FIGURES a b c Supplementary Figure 1 Fabrication of the nearfield radiative heat transfer device. a, Main fabrication steps for the bottom Si substrate. b, Main fabrication steps for the
More informationMAGNETOOPTIC IMAGING OF SINGLE VORTEX DYNAMICS IN NbSe 2 CRYSTALS
MAGNETOOPTIC IMAGING OF SINGLE VORTEX DYNAMICS IN NbSe 2 CRYSTALS M. Baziljevich, P. E. Goa, H. Hauglin, E. Il Yashenko, T. H. Johansen Dept. of Physics, University of Oslo, Box 1048 Blindern, 0316 Oslo,
More informationEmulsions Part 3. microemulsions miniemulsions. remarks to: Klaus Tauer MPI Colloids and Interfaces Am Mühlenberg, D Golm, Germany
Emulsions Part 3 remarks to: microemulsions miniemulsions Klaus Tauer MPI Colloids and Interfaces Am Mühlenberg, D14476 Golm, Germany Micro and Miniemulsion Why Special Emphasis? questionable graph!!!
More information